|Year : 2019 | Volume
| Issue : 4 | Page : 257-263
Comparison of self-adhering flowable composite microleakage with several types of bonding agent in class V cavity restoration
Atefeh Yousefi Jordehi, Maryam Shakur Shahabi, Alireza Akbari
Department of Operative Dentistry, School of Dentistry, Zanjan University of Medical Sciences, Zanjan, Iran
|Date of Web Publication||24-Jun-2019|
Dr. Maryam Shakur Shahabi
Department of Operative Dentistry, School of Dentistry, Zanjan University of Medical Sciences, Zanjan
Source of Support: None, Conflict of Interest: None
Background: The aim of the present study was to compare the marginal seal of self-adhering flowable composite resin with three universal bonding systems using the self-etch technique in Cl V cavities at enamel and dentin margins.
Materials and Methods: In this in vitro study, Cl V cavities were prepared on the buccal surfaces of forty premolars, with the occlusal margin of each cavity on enamel and gingival margin on dentin. The teeth were divided into four groups (n = 10) in terms of the adhesive used; Group 1: Vertise Flow (VF) self-adhering composite resin, Group 2: Clearfil S3 Bond Universal (CS3BU), Group 3: G-Premio Bond (GPB), Group 4: Single Bond Universal (SBU). In Groups 2, 3, and 4, Z350 flowable composite resin was used to restore the cavities. After thermocycling, the samples were immersed in 10% methylene blue for 24 h and evaluated under a stereomicroscope after buccolingual sectioning; microleakage at enamel and dentin margins was recorded. Kruskal–Wallis and Mann–Whitney tests were used for statistical analyses. Statistical significance was set at P < 0.5.
Results: Vertis Flow self-adhering composite resin exhibited significantly higher microleakage at enamel and dentin margins compared to SBU and CS3BU; however, it had significantly less microleakage at enamel margin compared to GPB (P < 0.05). At the enamel and dentin margins, the minimum microleakage values were recorded at SBU and CS3BU margins, respectively. GPB exhibited the highest microleakage values among the groups evaluated and in all the groups, microleakage at dentin and enamel margins was significantly different (P < 0.05) except for SBU group.
Conclusion: The marginal sealing ability of self-adhering flowable composite resin at enamel and dentin margins was poor compared to the majority of bonding agents evaluated.
Keywords: Adhesive, composite resin, dental leakage
|How to cite this article:|
Jordehi AY, Shahabi MS, Akbari A. Comparison of self-adhering flowable composite microleakage with several types of bonding agent in class V cavity restoration. Dent Res J 2019;16:257-63
|How to cite this URL:|
Jordehi AY, Shahabi MS, Akbari A. Comparison of self-adhering flowable composite microleakage with several types of bonding agent in class V cavity restoration. Dent Res J [serial online] 2019 [cited 2019 Nov 19];16:257-63. Available from: http://www.drjjournal.net/text.asp?2019/16/4/257/261129
| Introduction|| |
Simplification of bonding steps in composite resin restorations has been one of the most important aims of the development of dental adhesives. In addition to the simplification and shortening of the necessary time, decreasing and confinement of procedural errors has always been an aim for researchers. To this end, in recent years, single-bottle universal adhesives have been introduced, which can be applied in different self-etch, total etch and enamel selective etch modes. In addition, they can bond to different restorative materials, including metals and ceramics.,
Flowable composite resins were initially developed for use in Cl V cavities. However, nowadays they are used in different clinical procedures, including the restoration of small carious lesions, for sealing pits and fissures, and as liners for composite resin restorations. Flowable composite resins are easily placed in small cavities and they are expected to exhibit better adaptation with the cavity walls compared to composite resins with higher viscosity, Due to lower filler content, these composite resins have lower modulus of elasticity and higher polymerization shrinkage compare to conventional composite resin.
One of the recent advances in dentistry is the introduction of self-adhering flowable composite resins which are a product of combining an all-in-one bonding system and flowable composite resin. By the incorporation of glycero-phosphate dimethacrylate functional monomer into the chemical composition of composite resins, the steps of direct restorative procedures are simplified. Based on manufacturer's claim, this monomer exhibits acidic properties; it etches the tooth structure, bonds to the calcium of tooth structure, and has two functional methacrylate groups, which can copolymerize with other methacrylate monomers. Therefore, use of these composite resins results in shortening of the time needed to apply them and the procedural errors and technique sensitivity decrease. Based on previous studies, these composite resins have the highest elastic modulus, hardness, and degree of conversion compared to other conventional flowable composite resins. In addition, these composite resins exhibited higher hygroscopic dimensional expansion and more water sorption, compared to other flowable composite resins, 150 days after immersion in water.
Some studies have reported that selective etching with phosphoric acid and use of a bonding agent is effective for bonding ability of these composites to tooth structure.,, Different studies have compared the bonding ability of these composite resins to tooth structure with that of other bonding systems, reporting different results.,
Although clinical studies yield more valid results and use of in vitro findings has its specific limitations, laboratory tests are still useful for collecting initial data. One of these laboratory tests is microleakage test which is used for the evaluation of the sealing ability of materials. Poor seal and open margins is the main factor for marginal discoloration, recurrent caries and pulpal injury. Given the importance of the marginal seal of composite resin restorations, the aim of the preset study was to evaluate microleakage of flowable composite resin compared with universal bonding systems using the self-etch technique. Based on null hypothesis, there was no significant difference in the marginal sealing ability between self-adhering flowable composite resins and universal bonding systems.
| Materials and Methods|| |
The protocol of this in vitro present study was approved by the Ethics Committee of Zanjan University of Medical Sciences. Forty extracted teeth were selected and immersed in 0.5% chloramine solution at 4°C for almost 1 month before the study to prevent bacterial growth. All teeth were sound. The teeth with caries, restorations, trauma, enamel defects, and any congenital anomalies were excluded from the study.
Cl V cavities, measuring 2 mm in mesiodistal width, 2 mm occlusoginivally, and 1 mm in depth, were prepared on the buccal surface of each tooth with the use of a carbide fissure bur (010 SS White, Switzerland) under air and water spray using a high-speed handpiece. A periodontal probe was used to assess the accuracy of cavity dimensions. The cavities were prepared in a manner to place their center at the cemento-enamel junction; therefore, the occlusal margin was placed on the enamel and the gingival margin on the dentin or cementum. Finally, 0.5-mm bevel was placed on the enamel margin. A new bur was used for every 4 teeth.
The teeth were randomly assigned to four groups (n = 10) and conditioned with different universal bonding agents using the self-tech technique according to manufacturer's instructions and then restored with composite resin [Table 1]. For the purpose of matching, all the procedural steps were carried out by one operator.
- Group 1: Vertise Flow (VF) (Kerr, Orange, CA, USA)
- Group 2: Clearfil S3 Universal (Kuraray Noritake, Tokyo, Japan)
- Group 3: G-Premio Bond (GC, Tokyo, Japan)
- Group 4: Single Bond Universal (3M ESPE, St. Paul, MN, USA).
The samples in Groups 2–4 were restored with flowable Z350 Filtek composite resin (3M ESPE, St. Paul, MN, USA) after application of bonding agents. Light-curing was carried out with a halogen light-curing unit (Starlight Pro; Mectron s. p. a. Carasco, Italy, 1400 mw/cm2, 440–465 nm) in all the study groups. After restorative procedures, the restorations were polished and the samples were stored in distilled water at 27°C for 24 h.
Subsequently, the samples were subjected to a 500-cycle thermocycling procedure at 5/55°C with a dwell time of 30 s and a transfer time of 5 s. To carry out microleakage test, the apex of each tooth was sealed with sticky wax and all the tooth surfaces were covered with two layers of nail polish up to 1 mm from the cavity margins. Then all the samples were immersed in 10% methylene blue for 24 h. After retrieving the samples from the solution and rinsing them, the teeth were mounted in acrylic resin for better handling of the samples during sectioning. The mounted teeth were sectioned at the mid-sagittal area using a Mecatome machine (Pressi, France) under water cooling and evaluated under a stereomicroscope (Kyowa, Japan) at 50X at gingival and occlusal margins. For the purpose of blinding, evaluation of microleakage was carried out by a researcher who was unaware of the study groups. Microleakage at occlusal (enamel) and gingival (dentin) margins was classified as follows in terms of penetration of dye at restoration margins [Figure 1]:
|Figure 1: Dye penetration: Score 0 in enamel margin and score 2 in dentinal margin.|
Click here to view
- Score 0: No dye penetration
- Score 1: Dye penetration up to half of the cavity depth or less than that
- Score 2: Dye penetration up to more than half of the cavity depth without affecting the axial wall
- Score 3: Dye penetration to all the cavity walls with involvement of the axial wall.
Only the tooth side with maximum dye penetration at enamel or dentin margin was analyzed statistically. Nonparametric Kruskal–Wallis test was used to compare the 4 study groups at enamel and dentin margins. Mann–Whitney test was used to compare enamel and dentin margins in each group. Statistical significance was set at P < 0.5.
| Results|| |
Evaluation of enamel and dentin margins under a stereomicroscope revealed various degrees of microleakage [Table 2]. Statistical analyses showed significant differences in microleakage at enamel margins between the study groups (P < 0.05). The most frequent score at the enamel margin was score 1 in all the groups except Single Bond Universal group where score 1 (50%) was as same as score 0 (50%) [Figure 2].
|Table 2: Frequency distribution of microleakage scores in study groups, based on enamel and dentinal margins|
Click here to view
|Figure 2: Comparison of microleakage percentage between study groups in enamel margin.|
Click here to view
VF self-adhering composite resin exhibited significantly more microleakage at the enamel margin compared to Single Bond Universal and Clearfil S3 Bond Universal bonding systems; while it demonstrated significantly less microleakage at enamel margin compared to the G-Premio Bond group (P < 0.05). Based on the results at the enamel margin the decreasing scale of microleakage between the bonding systems was as follows: G-Premio Bond > Clearfil S3 Bond Universal > Single Bond Universal (P < 0.05).
There were significant differences in microleakage at the dentin margin between the study groups, except for VF and G-Premio Bond groups (P < 0.05). At the dentin margin score0 and score1 were the most common observation in all the groups except G-Premio Bond group where score0 was not observed at all [Figure 3].
|Figure 3: Comparison of microleakage percentage between study groups in dentinal margin.|
Click here to view
VF self-adhering composite resin exhibited significantly more microleakage at the dentin margin compared to Single Bond Universal and Clearfil S3 Bond Universal bonding systems. Among the study adhesives, the lowest microleakage score at the dentin margin was recorded in the Clearfil S3 Bond Universal group and the highest microleakage was observed in the G-Premio Bond group.
In each study group, microleakage was significantly different between the enamel and dentin margins except for the Single Bond Universal group (P < 0.05).
| Discussion|| |
Marginal seal is a key factor for the success of a restoration; it ensures the longevity of the restoration. Marginal seal depends on several factors, including the polymerization shrinkage, bonding to tooth structure, the elastic modulus of composite resin, thermal expansion coefficient of composite resin and its water sorption. Stresses resulting from polymerization of composite resin give rise to cracking of enamel prisms and marginal gaps; microleakage occurs due to the presence of these gaps around composite resin restorations.
In the present study, microleakage evaluation was used to study bonding systems and flowable composite resin. Cl V cavities were prepared with a high C-factor due to the high ratio of bonded surfaces-to-unbonded free surfaces. Thermocycling was applied to simulate thermal changes that occur in the oral cavity (500 cycles at 5/55°C) because thermal changes can affect microleakage. In addition, it has been shown that limited thermal cycles are adequate for the evaluation of microleakage, and microleakage increases with an increase in the number of thermal cycles in Cl V cavities.
Based on the results of the present study, there were significant differences in the marginal sealing ability between the study groups at enamel and dentin margins, refuting the null hypothesis of the study. This is consistent with the results reported by Vichi et al., who reported significant differences between the microleakage of all-in-one adhesive systems and self-adhering flowable composite resins in classic cavities; however, in their study, the marginal seal with self-adhering flowable composite resin was better than other bonding systems, which does not coincide with the results of the present study. In addition, another study showed that microleakage at dentin margins with the use of self-adhering flowable composite resin was more than that with the use of a 3-step etch-and-rise adhesive agent.
In contrast to the results of the present study, a study by Bektas et al. did not reveal any significant differences in microleakage between Vertise flowable composite resin and a self-etch all-in-one adhesive agent at enamel and dentin margins. In addition, another study did not show any significant differences in the enamel and dentin marginal seal between self-adhering flowable composite resin and different bonding systems.
In the present study, it was concluded that microleakage at enamel and dentin margins with the use of VF composite resin was more than that with the use of two other universal bonding systems in self-etch mode, except for G-Premio Bond system. This might be attributed to the poor wetting ability of this composite resin. Proper wetting ability of an adhesive agent on a substrate results in an intimate reaction between the substrate and the adhesive agent. Compared to other adhesive systems evaluated in the present study, VF has higher filler content and viscosity, no solvent and exhibits less wettability. These properties limit the ability of this material to penetrate into the exposed collagen network, despite the active use of the first layer of this material., Scanning electron microscope images have shown that this composite resin has a relatively superficial reaction with the tooth structure and does not form a clear hybrid layer. Due to such poor reaction between self-adhering flowable composite resins and tooth structures, several studies have reported that use of bonding agents increases the marginal seal of these composite resins at dentinal walls.,,
In the present study, universal bonding systems with the use of self-etch technique were compared with self-adhering flowable composite resin. One-step bonding systems have advantages such as simplifications, shortening of procedural steps and a decrease in technique sensitivity. Therefore, it was considered logical to make comparisons between universal adhesive systems in self-etch mode and VF composite resin.
The results of the present study showed significant differences in microleakage between different bonding systems at enamel and dentin margins, consistent with the results of the previous studies,, which might be attributed to differences in the chemical composition of these bonding agents.
Solvents are one of the most important components of universal bonding systems. The bonding systems evaluated in the present study were different from each other in relation to their solvents. Clearfil S3 Bond Universal and Single Bond Universal contain water and ethanol; according to the results they exhibited less microleakage compared to G-Premio Bond, which contains acetone. This is consistent with the results of previous studies which have reported a higher bonding ability in all-in-one adhesives containing a higher amount of ethanol., In addition, previous studies have shown that the acetone in G-Premio Bond might affect the formation of nano-layering through a change in the polarity of the solvent, with the subsequent hydrophobic effect of methacryloyloxydecyl dihydrogen phosphate (MDP) in the adhesive.
On the other hand, one of the monomers in the G-Premio Bond adhesive, which does not exist in the two other bonding systems, is 4-methacryloyloxyethy trimellitate anhydride, which is hydrolyzed to 4-methacryloyloxyethy trimellitate after its contact with water. This monomer greatly limits formation of nano-layering by 10-MDP-Ca salts.
Contrary to G-Premio Bond, Clearfil S3 Bond Universal and Single Bond Universal bonding systems contain 2- hydroxyethyl methacrylate monomer, which increases the wettability of the adhesivePrevious studies have shown less water drops in the hybrid layer formed by adhesives containing this monomer.,
It has been reported that pH can affect the bonding of bonding systems to the surface of dentin, too. In self-etch bonding systems, a pH value of >2 slows removal of minerals from the dentin surface and results in adequate time for the residual hydroxyapatite crystals to protect and open collagen fibers. The pH value in Clearfil S3 Bond Universal and Single Bond Universal is >2 and G-Premio Bond has a pH value of <2 [Table 1].
The amount of microleakage at enamel and dentin margins was significantly different in each study group except for the Single Bond Universal group. Since the microleakage of VF self-adhering flowable composite resin at enamel margin was more than that at the dentin margin, it appears etching the enamel surface before placing this composite resin is effective in decreasing microleakage., However, use of phosphoric acid on the dentin surface before placing self-adhering flowable composite resin might have a deleterious effect on the sealing ability of this composite resin due to excessive demineralization of the dentin surface and collapse of the collagen network.,
In the present study, since only the microleakage of self-etch universal boning systems and self-adhering flowable composite resin was evaluated, it is suggested that further studies be undertaken to evaluate the bond strength of universal bonding systems using different techniques and self-adhering flowable composite resins.
| Conclusion|| |
Under the limitations of the present study, the results showed that the marginal sealing ability of VF composite resin of enamel and dentin margins is not superior to that of other bonding agents evaluated. Therefore, caution should be exercise with the use of this composite resin without surface preparation or with the use of bonding agents. In this context, further studies are necessary to evaluate the efficacy of self-adhering flowable composite resins in the clinic.
This research has been supported by Zanjan University of Medical Sciences and Health Services grant for number A-11-1040-2 research proposal.
Financial support and sponsorship
Conflicts of interest
The authors of this manuscript declare that they have no conflicts of interest, real or perceived, financial or nonfinancial in this article.
| References|| |
Rengo C, Goracci C, Juloski J, Chieffi N, Giovannetti A, Vichi A, et al.
Influence of phosphoric acid etching on microleakage of a self-etch adhesive and a self-adhering composite. Aust Dent J 2012;57:220-6.
Perdigão J, Kose C, Mena-Serrano AP, De Paula EA, Tay LY, Reis A, et al.
Anew universal simplified adhesive: 18-month clinical evaluation. Oper Dent 2014;39:113-27.
Chen C, Niu LN, Xie H, Zhang ZY, Zhou LQ, Jiao K, et al.
Bonding of universal adhesives to dentine – Old wine in new bottles? J Dent 2015;43:525-36.
Amaral M, Belli R, Cesar PF, Valandro LF, Petschelt A, Lohbauer U, et al.
The potential of novel primers and universal adhesives to bond to zirconia. J Dent 2014;42:90-8.
Perdigão J, Sezinando A, Monteiro PC. Laboratory bonding ability of a multi-purpose dentin adhesive. Am J Dent 2012;25:153-8.
Bayne SC, Thompson JY, Swift EJ Jr., Stamatiades P, Wilkerson M. A characterization of first-generation flowable composites. J Am Dent Assoc 1998;129:567-77.
Unterbrink GL, Liebenberg WH. Flowable resin composites as “filled adhesives”: Literature review and clinical recommendations. Quintessence Int 1999;30:249-57.
Ikeda I, Otsuki M, Sadr A, Nomura T, Kishikawa R, Tagami J, et al.
Effect of filler content of flowable composites on resin-cavity interface. Dent Mater J 2009;28:679-85.
Baroudi K, Silikas N, Watts DC. Time-dependent visco-elastic creep and recovery of flowable composites. Eur J Oral Sci 2007;115:517-21.
Labella R, Lambrechts P, Van Meerbeek B, Vanherle G. Polymerization shrinkage and elasticity of flowable composites and filled adhesives. Dent Mater 1999;15:128-37.
Vichi A, Margvelashvili M, Goracci C, Papacchini F, Ferrari M. Bonding and sealing ability of a new self-adhering flowable composite resin in class I restorations. Clin Oral Investig 2013;17:1497-506.
Poss SD. Utilization of a new self-adhering flowable composite resin. Dent Today 2010;29:104-5.
Yuan H, Li M, Guo B, Gao Y, Liu H, Li J, et al.
Evaluation of microtensile bond strength and microleakage of a self-adhering flowable composite. J Adhes Dent 2015;17:535-43.
Salerno M, Derchi G, Thorat S, Ceseracciu L, Ruffilli R, Barone AC, et al.
Surface morphology and mechanical properties of new-generation flowable resin composites for dental restoration. Dent Mater 2011;27:1221-8.
Czasch P, Ilie N.In vitro
comparison of mechanical properties and degree of cure of a self-adhesive and four novel flowable composites. J Adhes Dent 2013;15:229-36.
Wei YJ, Silikas N, Zhang ZT, Watts DC. Hygroscopic dimensional changes of self-adhering and new resin-matrix composites during water sorption/desorption cycles. Dent Mater 2011;27:259-66.
Wei YJ, Silikas N, Zhang ZT, Watts DC. Diffusion and concurrent solubility of self-adhering and new resin-matrix composites during water sorption/desorption cycles. Dent Mater 2011;27:197-205.
Sadeghi M. An in vitro
microleakage study of class V cavities restored with a new self-adhesive flowable composite resin versus different flowable materials. Dent Res J (Isfahan) 2012;9:460-5.
Bektas OO, Eren D, Akin EG, Akin H. Evaluation of a self-adhering flowable composite in terms of micro-shear bond strength and microleakage. Acta Odontol Scand 2013;71:541-6.
Takeshi S, Junji K, Masayuki O, Junji T. Effect of cavity preparation with Er: YAG laser on marginal integrity of resin composite restoration. Asian Pac J Dent 2011;11:19-25.
De Munck J, Van Landuyt K, Peumans M, Poitevin A, Lambrechts P, Braem M, et al.
Acritical review of the durability of adhesion to tooth tissue: Methods and results. J Dent Res 2005;84:118-32.
Going RE. Microleakage around dental restorations: A summarizing review. J Am Dent Assoc 1972;84:1349-57.
Campanella LC, Meiers JC. Microleakage of composites and compomers in class V restorations. Am J Dent 1999;12:185-9.
Yazici AR, Celik C, Dayangac B, Ozgunaltay G. Effects of different light curing units/modes on the microleakage of flowable composite resins. Eur J Dent 2008;2:240-6.
Feilzer AJ, De Gee AJ, Davidson CL. Setting stress in composite resin in relation to configuration of the restoration. J Dent Res 1987;66:1636-9.
Gale MS, Darvell BW. Thermal cycling procedures for laboratory testing of dental restorations. J Dent 1999;27:89-99.
Wahab FK, Shaini FJ, Morgano SM. The effect of thermocycling on microleakage of several commercially available composite class V restorations in vitro
. J Prosthet Dent 2003;90:168-74.
Celik EU, Kucukyilmaz E, Savas S. Effect of different surface pre-treatment methods on the microleakage of two different self-adhesive composites in class V cavities. Eur J Paediatr Dent 2015;16:33-8.
Aguilar-Mendoza JA, Rosales-Leal JI, Rodríguez-Valverde MA, González-López S, Cabrerizo-Vílchez MA. Wettability and bonding of self-etching dental adhesives. Influence of the smear layer. Dent Mater 2008;24:994-1000.
Almaz ME, Oba AA, Sönmez IS, Sönmez D. Comparison of shear bond strength of self-adhering flowable composite with different flowable composites to dentin. Eur J Gen Dentistry 2016;5:6-10.
Margvelashvili M, Goracci C, Beloica M, Papacchini F, Ferrari M.In vitro
evaluation of bonding effectiveness to dentin of all-in-one adhesives. J Dent 2010;38:106-12.
Michor EL, Berg JC. Micellization behavior of aerosol OT in alcohol/water systems. Langmuir 2014;30:12520-4.
Tian F, Zhou L, Zhang Z, Niu L, Zhang L, Chen C, et al.
Paucity of nanolayering in resin-dentin interfaces of MDP-based adhesives. J Dent Res 2016;95:380-7.
Van Landuyt KL, De Munck J, Snauwaert J, Coutinho E, Poitevin A, Yoshida Y, et al.
Monomer-solvent phase separation in one-step self-etch adhesives. J Dent Res 2005;84:183-8.
Van Meerbeek B, Van Landuyt K, De Munck J, Hashimoto M, Peumans M, Lambrechts P, et al.
Technique-sensitivity of contemporary adhesives. Dent Mater J 2005;24:1-3.
Sadek FT, Calheiros FC, Cardoso PE, Kawano Y, Tay F, Ferrari M, et al.
Early and 24-hour bond strength and degree of conversion of etch-and-rinse and self-etch adhesives. Am J Dent 2008;21:30-4.
[Figure 1], [Figure 2], [Figure 3]
[Table 1], [Table 2]